practical method for diffusion welding of steel plate in air method for diffusion welding of steel...
Post on 06-Jul-2018
Embed Size (px)
NASA TECHNICAL NOTE
04 0 u= ro
n z c
PRACTICAL METHOD FOR DIFFUSION WELDING OF STEEL PLATE I N AIR
by Thomas J. Moore and Kenneth H. Holko
Lewis Research Center Cleueland, Ohio 44135
... .. KiRTLAND AFB, N.1
NATIONAL AERONAUTICS A N D SPACE ADMINISTRATION WASHINGTON, D. C. JULY 1971
TECH LIBRARY KAFB. NM
PRACTICAL METHOD FOR DIFFUSION WELDING 1I July 1971 OF STEEL PLATE I N AIR 7. Author(s)
Thomas J. Moore and Kenneth H. Holko
9. Performing Organization Name and Address
Lewis Research Center National Aeronautics and Space Administration Cleveland, Ohio 44135
12. Sponsoring Agency Name and Address
National Aeronautics and Space Administration Washington, D. C. 20546
15. Supplementary Notes
- -I 16. Abstract
6. Performing Organization Code
I 8. Performing Organization Report No. E-6236 10. Work Un i t No.
129-03 11. Contract or Grant No.i 13. Type of Report and Period Covered
Technical Note 14. Sponsoring Agency Code
In this report , a simple and easily applied method of diffusion welding steel plate in a i r is described. Feasibility was clearly established for the diffusion welding of butt joints in AIS1 1020 steel without the use of a vacuum furnace o r hot press . The diffusion welds equaled the strength of the parent metal and passed a 180Obend test. These results a r e believed to have considerable potential in basic industry and aerospace applications since elaborate vacuum hot presses and related equipment a r e not required to make the diffusion welds.
17. Key Words (Suggested by Author (s ) ) Metallic materials Unclassified - unlimited Machine element Diffusion welding
19. Security Classif. ( o f this report) 20. Security Classif. (o f th is page) 21. No. o f Pages 22. Price'
Unclassified Unclassified 25 $3.00
For sale b y t h e N a t i o n a l Technica l I n f o r m a t i o n Service, Spr ingf ie ld, V i rg in ia 22151
PRACTICAL METHOD FOR DIFFUSION WELDING OF STEEL PLATE IN AIR
by Thomas J. Moore and K e n n e t h H. Holko
Lewis Research Center
This work was designed to determine whether a simple and easily applied diffusion welding operation could be developed for thick steel plate. The novel feature of this welding method is that diffusion welds a r e made in air with deadweight loading. Another objective of this work was to examine the use of an autogenous (self-generated) surface-cleaning principle (termed "auto-vac cleaning") to reduce the effects of surface oxides that normally hinder diffusion welding.
A ser ies of nine butt joints were diffusion welded in thick sections (3. 8 to 5 . 1 cm, 1-2 1to 2 in. ) of AISI 1020 s teel plate. Diffusion welds were attempted at three welding
temperatures (1200, 1090, and 980' C) using a deadweight pressure of 3.45X104 N/m 2
(5 psi) and a 2-hour hold-time at temperature. Auto-vac cleaning operations prior to welding were also studied for the same three temperatures. Evaluation of weld quality was based on metallographic examination and room-temperature tensile and bend tests.
The results indicate that sound welds were produced at the higher two temperatures when the joints were previously fusion seal welded completely around the periphery. Also, auto-vac cleaning at 1200' C for 2-2
1 hours prior to diffusion welding was found to be highly beneficial, particularly when subsequent welding was accomplished at 1090' C.
This program is considered to be successful because sound diffusion welds were made in thick steel plate using simple procedures that can be readily applied in many industrial uses. Thus, the resul ts of this study a r e believed to have considerable potential in both aerospace and other industrial applications.
In this report , a simple and easily applied method of diffusion welding s teel plate in air is described. The feasibility of applying this welding method was clearly established
f o r AISI 1020 steel . The main purpose of this study was to devise a practical method of diffusion welding steel plate; that is, a procedure that does not require a vacuum furnace
or hot press . Another purpose was to gain information on the diffusion welding of a metal (steel) having an oxide that is unstable at elevated temperatures. Thus, information developed for the diffusion welding of steel is directly applicable to other metals that can absorb their oxides during the diffusion welding cycle. The results of this study a r e believed to have considerable potential in basic industrial as well as aerospace applications.
Kinzel (ref. 1)conducted early solid-state welding studies on the pressure welding of AISI 1020 s teel and other materials. Kinzel's technique involved pressure welding at temperatures between 800' and 1230' C, but the pressures were sufficient to produce measurable decreases in length. Therefore, these were solid-state deformation welds. Welds made at 1230' C were reported to be indistinguishable from the parent metal , with good tensile, bend, and impact properties. In the study reported herein, s imilar quality welds were produced at pressures low enough to prevent macrodeformation. (This solid-s ta te welding operation with no macrodeformation is termed diffusion welding (ref. 2). )
This program was of limited scope. For the initial portion of the study, two solid-state butt welds were made in 1.3-centimeter (0.5-in. ) diameter Type 304 stainless steel bar . Subsequently, nine butt welds were made in AISI 1020 steel plate, 3 .8 to 5.1 centimeters (1-
2 1to 2 in. ) thick, using a diffusion welding process. Welding temperatures
evaluated included 1200, 1090, and 980' C. Time at temperature was 2 hour, and the applied pressure was only 3.45X104 N/m 2 (5 psi).
An integral part of the diffusion welding operation was the use of an autogenous (selfgenerated) faying-surface cleaning principle. This cleaning principle has been described by Medovar (ref. 3) and Nikiforov (ref. 4). Medovar points out that for a steel assembly sea l welded at the periphery of the faying surfaces and heated to 1200' C for 1/2 hour, surface cleaning takes place autogenetically. After an initial pressure increase according to Charles ' law, a vacuum is formed within the sealed gap. Nikiforov visualizes that the oxygen within such a closed space is used up and further diffusion of metal ions to the surface enriches the surface with metal atoms. This was summed up as a peculiar process of dissolving oxides, which is possible in principle for any metal. Because of the fact that cleaning takes place autogenetically and a vacuum is theoretically produced in the gap, we have termed this process "auto-vac" cleaning.
Evaluation of weld quality was made on the basis of metallographic examination and room-temperature tensile and bend tests. All AISI 1020 steel weldments were exposed to a double-normalizing heat treatment prior to mechanical testing.
INITIAL STUDIES ON TYPE 304 STAINLESS STEEL BAR
In order to investigate the effectiveness of the auto-vac cleaning principle, two 1 .3 1centimeter-diameter by 3.8-centimeter (1/2-in. -diam by l--in. ) AIS1 Type 304 stainless2
steel bars were prepared for butt welding to produce a 7.6-centimeter (3-in.) long weldment, As shown in the outline in figure 1, the faying surfaces were ground (40. 7X10-6 cm r m s (16 rms)) and degreased in acetone just prior to seal welding at the joint periphery. The seal is the first s tep in preparing the assembly for auto-vac cleaning. The assembly after gas tungsten-arc (GTA) seal welding in helium is shown in figure 2. The machined flange served to minimize restraint on the weld bead and to minimize the heat input required for seal welding.
Electron-beam sea l welding was also investigated but showed no advantage over GTA based on metallographic examination of solid-state welded joints. In addition, seal welds were made by the shielded-metal-arc (SMA) welding process. Longer heating t imes were required to produce the auto-vac cleaning effect for the SMA seal-welded assemblies. Thus, it was decided to use GTA seal welding.
Auto-vac cleaning was applied to one of the GTA-sealed assemblies by heating to 1200' C for 1 hour in argon. (An air-atmosphere furnace would have been equally sufficient.) The second sealed assembly was not auto-vac cleaned (see fig. 1). Both assemblies were subsequently solid-state welded in an induction-heated vacuum hot press a s follows :
Temperature, O C . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 980 Pressure , N/m 2 (ksi) . . . . . . . . . . . . . . . . . . . . . . . 1.88X107 (2.73) Time at temperature, min . . . . . . . . . . . . . . . . . . . . . . . . . 5 Atmosphere, N/m 2 (torr) vacuum . . . . . . . . . . . . . . . . 2 . 7 ~ 1 0 - ~(2X10-5) Upset, mm (in.) decrease in length . . . . . . . . . . . . . . . . . . 0 .2 (0.008)
It should be noted here that since the joint periphery was sealed, the solid-state welds could have been made equally well in a i r . The vacuum hot press was used because it was readily available.
The beneficial effect of auto-vac cleaning prior to solid-state welding of Type 304 stainless steel is clearly shown in figure 3. With no auto-vac cleaning, a large amount of foreign material, believed to be principally chromium oxide, is concentrated near the weld line (fig. 3(a)). However, the weldment that was auto-vac cleaned shows little evidence of oxide at the w